General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.9 - 7.98 g/cm³ Show Material materials with Density of 7.9 - 7.98 g/cm³ |

50.0 °C | 7.96 g/cm³ Show Material materials with Density of 7.96 g/cm³ | |

100.0 °C | 7.94 g/cm³ Show Material materials with Density of 7.94 g/cm³ | |

150.0 °C | 7.92 g/cm³ Show Material materials with Density of 7.92 g/cm³ | |

200.0 °C | 7.9 g/cm³ Show Material materials with Density of 7.9 g/cm³ | |

250.0 °C | 7.88 g/cm³ Show Material materials with Density of 7.88 g/cm³ | |

300.0 °C | 7.86 g/cm³ Show Material materials with Density of 7.86 g/cm³ | |

350.0 °C | 7.83 g/cm³ Show Material materials with Density of 7.83 g/cm³ | |

400.0 °C | 7.81 g/cm³ Show Material materials with Density of 7.81 g/cm³ | |

450.0 °C | 7.79 g/cm³ Show Material materials with Density of 7.79 g/cm³ | |

500.0 °C | 7.76 g/cm³ Show Material materials with Density of 7.76 g/cm³ | |

550.0 °C | 7.74 g/cm³ Show Material materials with Density of 7.74 g/cm³ | |

600.0 °C | 7.71 g/cm³ Show Material materials with Density of 7.71 g/cm³ | |

650.0 °C | 7.68 g/cm³ Show Material materials with Density of 7.68 g/cm³ | |

700.0 °C | 7.66 g/cm³ Show Material materials with Density of 7.66 g/cm³ | |

750.0 °C | 7.63 g/cm³ Show Material materials with Density of 7.63 g/cm³ | |

800.0 °C | 7.61 g/cm³ Show Material materials with Density of 7.61 g/cm³ | |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa |

20.0 °C | 196 - 200 GPa Show Material materials with Elastic modulus of 196 - 200 GPa | |

50.0 °C | 197.57 GPa Show Material materials with Elastic modulus of 197.57 GPa | |

100.0 °C | 190 - 193.65 GPa Show Material materials with Elastic modulus of 190 - 193.65 GPa | |

150.0 °C | 189.43 GPa Show Material materials with Elastic modulus of 189.43 GPa | |

200.0 °C | 182 - 185 GPa Show Material materials with Elastic modulus of 182 - 185 GPa | |

250.0 °C | 180.11 GPa Show Material materials with Elastic modulus of 180.11 GPa | |

300.0 °C | 174 - 175.5 GPa Show Material materials with Elastic modulus of 174 - 175.5 GPa | |

350.0 °C | 170.89 GPa Show Material materials with Elastic modulus of 170.89 GPa | |

400.0 °C | 166 - 170 GPa Show Material materials with Elastic modulus of 166 - 170 GPa | |

450.0 °C | 162.26 GPa Show Material materials with Elastic modulus of 162.26 GPa | |

500.0 °C | 158 - 160 GPa Show Material materials with Elastic modulus of 158 - 160 GPa | |

550.0 °C | 154.02 GPa Show Material materials with Elastic modulus of 154.02 GPa | |

600.0 °C | 149.99 - 155 GPa Show Material materials with Elastic modulus of 149.99 - 155 GPa | |

650.0 °C | 146.07 GPa Show Material materials with Elastic modulus of 146.07 GPa | |

700.0 °C | 142 - 145 GPa Show Material materials with Elastic modulus of 142 - 145 GPa | |

750.0 °C | 138.32 GPa Show Material materials with Elastic modulus of 138.32 GPa | |

800.0 °C | 134 - 140 GPa Show Material materials with Elastic modulus of 134 - 140 GPa | |

900.0 °C | 127 - 135 GPa Show Material materials with Elastic modulus of 127 - 135 GPa | |

1000.0 °C | 120 - 125 GPa Show Material materials with Elastic modulus of 120 - 125 GPa | |

Unlock all property charts | ||

Elongation A80, transverse | 20.0 °C | 35 % Show Material materials with Elongation A80, transverse of 35 % |

Elongation, transverse | 20.0 °C | 35 % Show Material materials with Elongation, transverse of 35 % |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] |

50.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

100.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

150.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

200.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

250.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

300.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

350.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

400.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

450.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

500.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

550.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

600.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

650.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

700.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

750.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

800.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 77.01 - 78.09 GPa Show Material materials with Shear modulus of 77.01 - 78.09 GPa |

50.0 °C | 77.3 GPa Show Material materials with Shear modulus of 77.3 GPa | |

100.0 °C | 75.73 GPa Show Material materials with Shear modulus of 75.73 GPa | |

150.0 °C | 73.87 GPa Show Material materials with Shear modulus of 73.87 GPa | |

200.0 °C | 71.91 GPa Show Material materials with Shear modulus of 71.91 GPa | |

250.0 °C | 69.95 GPa Show Material materials with Shear modulus of 69.95 GPa | |

300.0 °C | 67.89 GPa Show Material materials with Shear modulus of 67.89 GPa | |

350.0 °C | 65.83 GPa Show Material materials with Shear modulus of 65.83 GPa | |

400.0 °C | 63.96 GPa Show Material materials with Shear modulus of 63.96 GPa | |

450.0 °C | 62.1 GPa Show Material materials with Shear modulus of 62.1 GPa | |

500.0 °C | 60.33 GPa Show Material materials with Shear modulus of 60.33 GPa | |

550.0 °C | 58.57 GPa Show Material materials with Shear modulus of 58.57 GPa | |

600.0 °C | 56.9 GPa Show Material materials with Shear modulus of 56.9 GPa | |

650.0 °C | 55.33 GPa Show Material materials with Shear modulus of 55.33 GPa | |

700.0 °C | 53.86 GPa Show Material materials with Shear modulus of 53.86 GPa | |

750.0 °C | 52.29 GPa Show Material materials with Shear modulus of 52.29 GPa | |

800.0 °C | 50.82 GPa Show Material materials with Shear modulus of 50.82 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 510 - 690 MPa Show Material materials with Tensile strength of 510 - 690 MPa |

50.0 °C | 493 MPa Show Material materials with Tensile strength of 493 MPa | |

100.0 °C | 465 MPa Show Material materials with Tensile strength of 465 MPa | |

150.0 °C | 440 MPa Show Material materials with Tensile strength of 440 MPa | |

200.0 °C | 420 MPa Show Material materials with Tensile strength of 420 MPa | |

250.0 °C | 400 MPa Show Material materials with Tensile strength of 400 MPa | |

300.0 °C | 385 MPa Show Material materials with Tensile strength of 385 MPa | |

350.0 °C | 375 MPa Show Material materials with Tensile strength of 375 MPa | |

400.0 °C | 370 MPa Show Material materials with Tensile strength of 370 MPa | |

450.0 °C | 360 MPa Show Material materials with Tensile strength of 360 MPa | |

500.0 °C | 350 MPa Show Material materials with Tensile strength of 350 MPa | |

550.0 °C | 340 MPa Show Material materials with Tensile strength of 340 MPa | |

600.0 °C | 320 MPa Show Material materials with Tensile strength of 320 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 20.0 °C | 510 - 690 MPa Show Material materials with Tensile strength, transverse of 510 - 690 MPa |

Yield strength Rp0.2 | 50.0 °C | 191 MPa Show Material materials with Yield strength Rp0.2 of 191 MPa |

100.0 °C | 175 MPa Show Material materials with Yield strength Rp0.2 of 175 MPa | |

150.0 °C | 166 MPa Show Material materials with Yield strength Rp0.2 of 166 MPa | |

200.0 °C | 157 MPa Show Material materials with Yield strength Rp0.2 of 157 MPa | |

250.0 °C | 147 MPa Show Material materials with Yield strength Rp0.2 of 147 MPa | |

300.0 °C | 137 MPa Show Material materials with Yield strength Rp0.2 of 137 MPa | |

350.0 °C | 132 MPa Show Material materials with Yield strength Rp0.2 of 132 MPa | |

400.0 °C | 128 MPa Show Material materials with Yield strength Rp0.2 of 128 MPa | |

450.0 °C | 123 MPa Show Material materials with Yield strength Rp0.2 of 123 MPa | |

500.0 °C | 118 MPa Show Material materials with Yield strength Rp0.2 of 118 MPa | |

550.0 °C | 118 MPa Show Material materials with Yield strength Rp0.2 of 118 MPa | |

600.0 °C | 113 MPa Show Material materials with Yield strength Rp0.2 of 113 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 200 MPa Show Material materials with Yield strength Rp0.2, transverse of 200 MPa |

Yield strength Rp1.0 | 50.0 °C | 227 MPa Show Material materials with Yield strength Rp1.0 of 227 MPa |

100.0 °C | 205 MPa Show Material materials with Yield strength Rp1.0 of 205 MPa | |

150.0 °C | 195 MPa Show Material materials with Yield strength Rp1.0 of 195 MPa | |

200.0 °C | 186 MPa Show Material materials with Yield strength Rp1.0 of 186 MPa | |

250.0 °C | 176 MPa Show Material materials with Yield strength Rp1.0 of 176 MPa | |

300.0 °C | 167 MPa Show Material materials with Yield strength Rp1.0 of 167 MPa | |

350.0 °C | 162 MPa Show Material materials with Yield strength Rp1.0 of 162 MPa | |

400.0 °C | 157 MPa Show Material materials with Yield strength Rp1.0 of 157 MPa | |

450.0 °C | 152 MPa Show Material materials with Yield strength Rp1.0 of 152 MPa | |

500.0 °C | 147 MPa Show Material materials with Yield strength Rp1.0 of 147 MPa | |

550.0 °C | 147 MPa Show Material materials with Yield strength Rp1.0 of 147 MPa | |

600.0 °C | 142 MPa Show Material materials with Yield strength Rp1.0 of 142 MPa | |

Unlock all property charts | ||

Yield strength Rp1.0, transverse | 20.0 °C | 240 MPa Show Material materials with Yield strength Rp1.0, transverse of 240 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.63E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.63E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.69E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.69E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.73E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.73E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.78E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.78E-5 - 1.81E-5 1/K | ||

500.0 °C | 1.82E-5 - 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.82E-5 - 1.84E-5 1/K | ||

600.0 °C | 1.85E-5 - 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.85E-5 - 1.88E-5 1/K | ||

700.0 °C | 1.87E-5 - 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.87E-5 - 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 2E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 800 °C Show Material materials with Max service temperature, long of 0 - 800 °C | ||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 450 - 472 J/(kg·K) Show Material materials with Specific heat capacity of 450 - 472 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 13.3 - 17 W/(m·K) Show Material materials with Thermal conductivity of 13.3 - 17 W/(m·K) | |

100.0 °C | 14.9 W/(m·K) Show Material materials with Thermal conductivity of 14.9 W/(m·K) | ||

200.0 °C | 16.5 W/(m·K) Show Material materials with Thermal conductivity of 16.5 W/(m·K) | ||

300.0 °C | 18.1 W/(m·K) Show Material materials with Thermal conductivity of 18.1 W/(m·K) | ||

400.0 °C | 19.5 W/(m·K) Show Material materials with Thermal conductivity of 19.5 W/(m·K) | ||

500.0 °C | 21 W/(m·K) Show Material materials with Thermal conductivity of 21 W/(m·K) | ||

600.0 °C | 22.4 W/(m·K) Show Material materials with Thermal conductivity of 22.4 W/(m·K) | ||

700.0 °C | 23.8 W/(m·K) Show Material materials with Thermal conductivity of 23.8 W/(m·K) | ||

800.0 °C | 25.2 W/(m·K) Show Material materials with Thermal conductivity of 25.2 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.5 mm²/s Show Material materials with Thermal diffusivity of 3.5 mm²/s | |

100.0 °C | 3.8 mm²/s Show Material materials with Thermal diffusivity of 3.8 mm²/s | ||

200.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

300.0 °C | 4.3 mm²/s Show Material materials with Thermal diffusivity of 4.3 mm²/s | ||

400.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

500.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

600.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

700.0 °C | 5.1 mm²/s Show Material materials with Thermal diffusivity of 5.1 mm²/s | ||

800.0 °C | 5.4 mm²/s Show Material materials with Thermal diffusivity of 5.4 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.1E-7 - 7.91E-7 Ω·m Show Material materials with Electrical resistivity of 7.1E-7 - 7.91E-7 Ω·m |

50.0 °C | 7.61E-7 Ω·m Show Material materials with Electrical resistivity of 7.61E-7 Ω·m | |

100.0 °C | 7.99E-7 - 8.45E-7 Ω·m Show Material materials with Electrical resistivity of 7.99E-7 - 8.45E-7 Ω·m | |

150.0 °C | 8.38E-7 Ω·m Show Material materials with Electrical resistivity of 8.38E-7 Ω·m | |

200.0 °C | 8.72E-7 - 9.19E-7 Ω·m Show Material materials with Electrical resistivity of 8.72E-7 - 9.19E-7 Ω·m | |

250.0 °C | 9.04E-7 Ω·m Show Material materials with Electrical resistivity of 9.04E-7 Ω·m | |

300.0 °C | 9.34E-7 - 9.77E-7 Ω·m Show Material materials with Electrical resistivity of 9.34E-7 - 9.77E-7 Ω·m | |

350.0 °C | 9.63E-7 Ω·m Show Material materials with Electrical resistivity of 9.63E-7 Ω·m | |

400.0 °C | 9.91E-7 - 1.03E-6 Ω·m Show Material materials with Electrical resistivity of 9.91E-7 - 1.03E-6 Ω·m | |

450.0 °C | 1.02E-6 Ω·m Show Material materials with Electrical resistivity of 1.02E-6 Ω·m | |

500.0 °C | 1.04E-6 - 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.04E-6 - 1.08E-6 Ω·m | |

550.0 °C | 1.06E-6 Ω·m Show Material materials with Electrical resistivity of 1.06E-6 Ω·m | |

600.0 °C | 1.08E-6 - 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 - 1.12E-6 Ω·m | |

650.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

700.0 °C | 1.12E-6 - 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 - 1.15E-6 Ω·m | |

750.0 °C | 1.14E-6 Ω·m Show Material materials with Electrical resistivity of 1.14E-6 Ω·m | |

800.0 °C | 1.15E-6 - 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 - 1.18E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.04 - 0.1 % Show Material materials with Carbon of 0.04 - 0.1 % |

Chromium | 15 - 17 % Show Material materials with Chromium of 15 - 17 % |

Manganese | 1.5 % Show Material materials with Manganese of 1.5 % |

Nickel | 12 - 14 % Show Material materials with Nickel of 12 - 14 % |

Niobium | 1.2 % Show Material materials with Niobium of 1.2 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.3 - 0.6 % Show Material materials with Silicon of 0.3 - 0.6 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Titanium | 1.2 % Show Material materials with Titanium of 1.2 % |